- Email: [email protected]

~

Pergamon

0956-7151(94)E0112-T

Copyright © 1994 Elsevier Science Ltd Printed in Great Britain. All rights reserved 0956-7151/94 $7.00 + 0.00

DENSIFICATION A N D CREEP IN THE FINAL STAGE OF SINTERING H. RIEDELt, V. KOZAK2 and J. SVOBODAz ~Fraunhofer-Institut for Werkstoffmechanik, W6hlcrstrabe 11, D-79108 Freiburg, Germany and 2Institute of Physical Metallurgy, Academy of Sciences of the Czech Republic, Zizkova 22, 61662 Brno, Czech Republic

(Received 9 August 1993; in revisedform 19 January 1994) Abstract--Densification and creep by grain boundary diffusion is modelled for the late stage of sintering. The grain structure is described as a regular array of tetrakaidekahedra with pores at each grain boundary between next-nearest neighbors. The diffusion problem on the surface of the tetrakaidekahedron is solved numerically using the heat-conduction option of the finite element code ANSYS. From the calculated normal stresses on the boundary facets one assembles the macroscopic constitutive behavior. Since the assumed grain shape is the Wigner-Seitz cell of the body-centered cubic lattice, the resulting viscosity tensor has cubic symmetry. Isotropic bulk and shear viscosities are obtained by applying the procedures developed for the elasticity theory of polycrystals. The resulting bulk viscosity is well approximated by a closed-form solution developed previously. Due to the pronounced cubic anisotropy of the model, the isotropic shear viscosity cannot be determined unambiguously. The model includes the effect of viscous grain boundary sliding. The influence of surface diffusion on the sintering rate is also explored.

1. INTRODUCTION The uniaxial pressing of ceramic or metallic powders generally leads to powder compacts with inhomogeneous density distributions. Such inhomogeneities result in shape distortions during sintering. There have been attempts to predict the shape of the sintered part by finite element simulation of the pressing and sintering processes with the goal of adjusting the shape of the pressing tools and the pressing schedule such that the final part assumes the required shape (e.g. [1~5]). The shape evolution during sintering may depend sensitively on the constitutive behavior under multiaxial stresses. Especially, if the sintering material can be described as linear viscous, the ratio of the shear to the bulk viscosity, G/K, is an important factor. Classical sintering theories (e.g. [7-9]) are usually not concerned with the question of shear loading of material elements and hence do not provide estimates of the shear viscosity G. Only recently the problem was addressed in connection with the desire to analyze stresses and distortions during inhomogeneous sintering, either for simple goemetries [10-13] or for complex parts [1--6]. In this paper, a model for closed porosity is presented with grain boundary diffusion being the assumed transport mechanism. This is justified for fine-grained materials at not too high temperatures, and in the absence of liquid phases. Grain boundary sliding is described by a linear relation between shear stress and sliding speed. Surface diffusion on the pore surfaces is assumed to be fast enough that the pores

develop near-equilibrium shapes after pore closure. However, the free energy dissipated by surface diffusion is taken into account in the thermodynamic balance equation. The resulting retardation of sintering is treated in Section 6. Since grain boundary diffusion is governed by a linear relation between displacement rate and stress, the macroscopic constitutive equation will be a linear viscous law. In the isotropic case the general form is O"~]

~ij= ~

O"m - - O"s

+ 6,j

3K

(1)

Here, i;j and a;j are the strain rate and stress tensors, the prime denotes the deviator, o"m is the mean (or hydrostatic) stress, as is the sintering stress, 6;j is the Kronecker symbol, and G and K are the shear and bulk viscosities, respectively. The aim of a micromechanical model is to specify G, K, as, which depend on the relative density p, on the dihedral angle ~ and on the arrangement of the grains. The dihedral angle is defined by cos ~O= 7b/(2ys), where L and 7b are the surface the grain boundary energies per unit area, respectively. Micromechanical models were developed for open porosity by various working groups assuming either viscous flow of the grains [14, 15] or grain boundary diffusion [16-18] as the governing transport mechanism. The G/K ratio is obtained by these models as 0.6, if the particle contacts are randomly oriented and if they have no spatial correlation. If there is a shortrange order in the particle arrangement, for example a body-centered cubic particle packing over small

3093

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING

3094

distances, the G/K ratio is found to be smaller, and a value of 0.27 was advocated in [18]. Experimental values tend to be larger and often exceed the value 0.6, which is considered to be an upper bound in the models. This is an unresolved problem. For closed porosity, a three-dimensional model for sintering and diffusion creep was developed by Pan and Cocks [19] using a bounding theorem. Similarities and differences between their:model and the present model will be pointed out in the following sections. One of the main differences is that Pan and Cocks ignore the cubic anisotropy of the model and derive the shear response for a special orientation only. In this paper, the full anisotropic response is derived and averaging methods are applied to find isotropic averages for the shear viscosity. 2. DESCRIPTION OF THE MODEL

gradient operator, a n is the normal component of the stress acting on the grain boundary, f~ is the atomic volume, 6D b is the grain boundary diffusion coefficient, k is the Boltzmann constant and T is the absolute temperature. The summation convention is applied for repeated vector and tensor indices i, j in equation (3) and in the rest of the paper.

2.3. Grain boundary sliding Grain boundary sliding at a rate St is assumed to result in a tangential force F t = r/At~t

(5)

where A is the area of the grain facet (excluding the area occupied by pores) and ~/is a viscosity coefficient for sliding. In Section 4, the effect of viscous grain boundary sliding is neglected, but it will be included in Section 5. 3. THE SINTERING STRESS

2.1. Geometry The pore configuration analyzed in this paper is shown in Fig. 1(a) in comparison with the one studied by Pan and Cocks [19] [Fig. l(b)]. Both approaches use a periodic, body-centered cubic (b.c.c.) array of tetrakaidekahedral grains, but Pan and Cocks place the pores on the 24 grain corners, while we consider pores on the six square facets of the grains. Their choice corresponds to the classical picture [7], while ours is motivated by the investigation of equilibrium shapes of the open pore space and the evolution of the pores at the transition to closed porosity [17].

2.2. Grain boundary diffusion Grain boundary diffusion is described by the equations

Ji=

6Db k T V~trn

V~j~ = - a a V2a. -

kT - t~. fl 6D b

(2) (3) (4)

where the first gives the vector of the flux density, Ji, as a function of the gradient of the chemical potential, ['~O'n, the second is the continuity equation and the third follows by combining the previous two. The symbols a r e : /~n is the relative displacement rate of touching grains normal to the contact area, V~ is the

The sintering stress, as, can be calculated in advance without solving the diffusion problem. A preliminary expression for the sintering stress was derived in [17] for the present configuration. However, since [17] was concerned primarily with open porosity, an inaccuracy in the derivation of the sintering stress for closed pores on two-grain junctions remained undetected. A porous polycrystalline solid is in equilibrium, if the applied mean stress, which is then called the sintering stress, balances the internal surface and interface tension forces tTsdV = 7b dAb + 7s dA~

(6)

where d V is a virtual change of the volume of the unit cell, and dAb and dAs are the associated changes of the grain boundary area and surface area, respectively. For one unit cell Ab= 4A6+ 3.44 and A s = 3Ap, where A6, A 4 and .4p are the areas of one hexagonal and one square facet and of the surface of one pore, respectively. After division of equation (6) by dt one obtains time derivatives, which are given by the geometrical relations ,46 = 3x//3a2~m

"44 = 2a2~m -- 2~ sin 2 ~ri A~ = 24~(1 -- cos ~b)r? ~" :

3 VE m .

(7)

Here Em is the mean strain rate, a is the edge length of the tetrakaidekahedron, which is related to its volume by V --- 8x/2a 3, and r is the radius of curvature of the pore surface, which is related to the volume of one pore, Vp, by 2~z Vp = Fv(~)r 3with Fv = -~- (2 -- 3 cos ~b + cos 3 ~,). Fig. 1. Alternative configurations of closed porosity. (a) Present work, (b) Pan and Cocks [19].

(8)

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING With these relations equation (6) yields the sintering stress

27', ( 9 F v p p),/3 . 2V/~+ a,=~-\~-~ 1-- . - t - ~ ~ - j

1 //3p'~'/3yb

~.

corresponding nj, and their magnitude, for the hexagonal and square facets, respectively, is

]rj] = - 2R

(9)

Here the relative density, p, was introduced, which is related to the pore volume by 1 - p = 3 Vp/ V; R is the radius of the sphere having the same material volume as a grain, i.e. V = (4~/3)R3/p. In [17] the second term is missing from equation (9). This term results from the fact that the surface of the whole unit cell shrinks during densification, while the first term accounts for the changes of the surface and grain boundary areas at the pore tip. 4. SOLUTION OF THE DIFFUSION PROBLEM

4.1. Overview The diffusion problem on the surface of the tetrakaidekahedron is solved in the following way. The macroscopic strain rate tensor is considered to be known. Four different cases of prescribed straining are treated in the (numerical) analysis. From the strain rate the normal displacement rates on the grain boundary facets are calculated. Further, the smallest possible unit cells for the solution of the diffusion equation (4) are identified and boundary conditions are specified. Then equation (4) is solved numerically using the heat-conduction option of the finite-element program ANSYS. The normal displacement rate is analogous to the heat production rate, the normal stress is analogous to the temperature, and ~ &Db/kT plays the role of the thermal conductivity. The finite element program generates solutions for the distribution of the normal stress, a n. Integrating (numerically) over the facets gives the forces transmitted by each facet. From these forces the macroscopic viscosity tensor is assembled by the same method that was applied for open porosity in [15, 18]. Finally the cubic viscosities are averaged to obtain isotropic values.

Irjl

ftn = nirj~ij

(10)

where rj is the vector connecting the grain centres. The macroscopic strain rate tensor is considered to be prescribed. The response of the material in terms of stress is calculated in the following section. The cubic axes of the tetrakaidekahedron are normal to the square facets, and we choose a Cartesian coordinate system aligned with the cubic axes. Then the normal unit vectors on the square facets are {100}, and those on the hexagonal facets are (l/x/3) { 111 }. The notation with the parentheses implies all possible permutations of the components including + 1 and - 1 . The vectors rj are all parallel to the AMM 42/9--M

(11)

,/3\p]

'j3 .

(12)

Here P0 is the density of the b.c.c, sphere packing, i.e. P0 = n ~/3/8 = 0.68. For p = P0 the distance between nearest neighbor spheres is 2R, and that between next-nearest neighbors in 2/x/3 times larger.

4.3. Loading cases The numerical calculations of the diffusion fields on the surface of the tetrakaidekahedron are performed for the following four loading cases. (I) Unidirectional extension in [001] direction. In this case the only nonzero strain rate component is £33- The aim is to calculate the stresses needed to cause this strain rate. Equation (10) gives the normal displacement rates on the grain facets. The result, together with those of the other loading cases, will be summarized at the end of this section. The diffusion equation (4) is solved numerically with these prescribed displacement rates on the unit cell shown in Fig. 2. It comprises a quarter of a hexagonal facet, a quarter of a square facet with (100) orientation and an eighth of the square facet with (001) orientation. These facets are shown in Fig. 3 tilted into the plane of drawing. The circular arcs represent the edges of the pores, which were omitted from Fig. 2 for simplicity. The unit cell is chosen such that, because of the symmetry of the problem, no matter flows across the outer boundary, except into the pores. At the edge of the pores, continuity of the chemical potential demands that tr, = 2~,/r. This stress is set equal to zero in the computation since it leads to an additive X3

4.2. Displacement rates The normal displacement rate on a grain contact area with unit normal vector n i is given by

3095

!

[001] ELL ~SES 14 INITCELL ORCASE2 I

[0101 X2

Fig. 2. Unit ceils for the treatment of the diffusion problems.

3096

R I E D E L et al.:

DENSIFICATION

~-

On=O

''',,,,,

2(~D b

D b ',,, (sql) ",,,,,

2Cl(hex) n

.

.

On = 0

.

.

IN THE FINAL STAGE OF SINTERING

Jn -- 0

.

.. (sq3',

(~Db .. (hex) UR

Fig. 3. U n i t cell for loading case (1). All facets are s h o w n

in one plane. term, the sintering stress, which is already known from equation (9). Further, at the border line between hexagonal and square facets the normal components of the flux density must obey j~q) + 2j~ ~) = 0, since at each edge of the grain two equivalent hexagonal facets meet with one square facet. In the numerical model this requirement is met by doubling the "thickness" of the hexagonal facet, i.e. by artificially doubling 6Db and u,. Then the flux density is continuous and the stress is calculated correctly. The resulting forces on the grain facets and the cubic moduli are given later. (2) Shear on (100) planes in [010] direction. The only nonzero strain rate and stress components are now ~12 = ~2~ and try2= ~r2~. The resulting displacement rates are obtained from equation (10) and they are listed at the end of this section. The unit cell for the numerical solution of the diffusion equation must be larger than in the previous loading case. It is shown in Fig. 2 and, plotted on a plane, in Fig. 4. It comprises one half of a hexagonal facet, a quarter of the square facet with (100) orientation, and one eighth of the square facet with (001) orientation. At the triple grain junctions, the flux does not branch in this loading case, but flows continuously from one facet to one of the others, while the third does not exchange matter with the first two. The boundaries on the right and at the bottom of Fig. 4 are characterized by zero normal flux, while at the boundaries on the left ~ = 0 because of the symmetry of the loading. At the edges of the pores, one prescribes a, = 0 also. (3) Isostatic loading. Isostatic loading with a mean strain rate ~m= ~t = ~22 = ~33 leads to a hydrostatic stress state with mean stress ~rm. This loading case could be obtained by superposition from case (1), so that a separate numerical analysis would not be necessary. However, the redundance in numerical calculations can be used to test their consistency. In fact, the bulk moduli calculated from loading cases (1) and (3) agree to within 0.01%. In the numerical calculation the same unit cell was used as in loading case (1), although a smaller cell would have been sufficient because of the higher symmetry.

~D b ',,,

0~sq 1) ',,,,

Fig. 4. Unit cell for loading case (2). All facets are shown in one plane.

(4) Creep in [001] direction without pores. In the absence of pores, loading cases (1) and (3) cannot be prescribed since the material is incompressible, in this case, we prescribe the strain rate components E33 = --2Eli-~" --2E22' The unit cell for the finite element calculation is the same as in loading case (1). An arbitrary stress value can be prescribed at any location and we choose an = 0 in the center of the square facets with normals in Xl and x2 directions. The choice of the stress boundary condition specifies the hydrostatic stress, which, however, plays no role for deviatoric creep. Summary of the displacement rates. The displacement rates following from equation (10) for the four loading cases are given in Table 1 in nondimensional form, ~n, which is defined by ~n = ~ n 2 R ( ~ ) 1/3,

(13)

where ~ means Ea3, ~2, £m and E3a in cases (1), (2), (3) and (4), respectively.

4.4. Finite element solution Figure 5 shows the grids used in the finite element solution of the diffusion equation (4) with the ti,values and boundary conditions specified in the preceding section. Eight-noded isoparametric quadrilaterals are used with 3 x 3 integration points. Table 1. Dimensionless displacement rates on square facets with normals in %-direction (sq3) or in xl- or x2-directions (sql) or (sq2), and on hexagonal facets (hex) ~q3)

a~ql) = ,;~q2)

(1) ~33~ 0

Loading case

2/~/3

0

a~ex)

1/3

(2) ~n ~ 0 (3) ~md: 0 (4) ~33= - 2 i .

0 2/x/3 2/~/3

0 2/x/3 --1/43

__.2/3 1 0

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING

3097

a)

Fig. 5. Finite element grids on the unit cells. Computations were carried for four different pore sizes rp/(x/2a ) = 0, 0.1, 0.2 and 0.3; rp is the pore radius in the grain boundary. Table 2 gives the corresponding values of the area fraction of the square gain facets covered by pores, oJ = nrZp/a2, and the corresponding relative densities, p; p and co are related by co = ~ s i n 2

I//(.8 x//23(~lFv-P ))2/3.

(14)

Figure 6 shows the distribution of the normal stress, an, on the grain boundaries. The stress is given in units of kTR3~./(f~ 6Dbp). The iso-stress lines correctly exhibit kinks, where they intersect triple grain lines with discontinuities in 6D b and tin. The flux vector is normal to the isostress lines. Considering the isostatic case [Fig. 6(c)], the isostress lines are nearly circular, so that the flow is approximately radial around the centers of the square and hexagonal facets. Hence the approximation of radial flow made in [18] is expected to yield good estimates for the bulk viscosity (see Section 5.3). Figure 6(d) shows the stress distribution under creep conditions in the absence of pores. Again the flow pattern on the square facet normal to the tensile axis is nearly radial. Contrary to this (numerical) observation, Pan and Cocks [19] assume a parallel flow field to describe deviatoric creep. Hence it is not surprising that their result for the strain rate is found Table 2. Area coverage, co, and relative density, p, for which the finite element calculationsare carried out rp/a co p (for ~O= 60°) p (for ¢, = 90°) 0 0 I I 0.1~2 0.0628 0.9985 0.9969 0.2~2 0.2513 0.9879 0.9749 0.3x/2 0.5655 0.9592 0.9152

to differ markedly from the numerical result shown below. Table 3 shows the dimensionless forces on the boundary facets, which are obtained by integration of the stress over the facets. The nondimensional force jO,, is defined by (~)2/3 kTRSg

F. = F,

(15)

n fiDbp

where g has the same meaning as before, namely g33, ~2, gr. and g33 in the four loading cases. The slight difference of the order 0.1% between sq3 and sql in the isostatic case arises from the asymmetry of the finite element grid. It can be considered as a measure of the accuracy of the finite element results.

4.5. Macroscopic stresses and viscosities The macroscopic stresses are calculated most easily by equating the work rates (per volume) done by the macroscopic stresses and by the contact forces

trijgiJ = 1 g, F~k)ti~k) 2V~

"

" '

(16)

Here V = ( 4 n / 3 ) R 3 / p is the volume of the tetrakaidekahedron, including the pore space, the sum extends over all facets of the grain, and the factor 1/2 is needed since each facet is shared by two grains. The work rate on the left-hand side of equation (16) can be written as ag, where 0- means o33, 2trl2 , 30-m and 0-33--O'11 in the four loading cases, and was given earlier. Using the dimensionless forms of Fn and zin in equation (16) and dividing by ~ gives the stress F3v/3

kTR3 7.

3098

RIEDEL et aL:

DENSIFICATION IN THE FINAL STAGE OF SINTERING

a) Case 1

b) Cas o O.Ol 4 0.028 0.042 0.056 0.07

o.o,49

0.035 0.021 -

0.084 0.063

0.098 0.112 0.126

0.056

0.049

0.14

0.035 0.021 0

c)

d)

0.168

o.o35 •

0.14

0.0 4

0.042 0.049

.02

0.056

0.112 0.056

0.063

0

\

Fig. 6. Lines of constant normal stress for the loading cases (1)-(4). The lines are equidistant in stress. where 0" and ~ have the above meaning. The term in square brackets specifies the viscous moduli, as shown next. For cubic anisotropy, the linear viscous relations are

0"12 = 2C44E12

(19)

0"m=3g~m

(20)

0"33 - - 0"11 = 3 ( C l l _ C12)~33 0"33 ~" Cl1E33

(18)

0"11 = CI2E33

Table 3. Dimensionlessnormal forces on grain facets Loading case

rp/a

p~3)

ptml), _--p(m21,

p~ex)

(1) Uniaxial extension (~33 ~ 0)

0.1x~2 0.2~,2 0.3~/2

0.140405 0.046543 0.009184

0.120572 0.038928 0.007761

0.528873 0.271125 0,129573

(2) Shear (i12~ 0)

0 0 0.1x~2 0 0.2~2 0 0.3,~/2 0 (3) lsostatic 0.1x/2 0.381398 0.2~2 0.124438 0.3x/2 0.024694

0 0 0 0 0.381631 0.124375 0.024712

(4) Creep in x 3 direction

0.014112

0

0.096127

± 0.,149787 ± 0.435817 ± 0.393674 ± 0.323005 1.586608 0.813366 0.388726 0.107621

(21)

for the four loading cases, respectively. The C0's are the cubic viscosities, and K = (Clt + 2C12)/3 is the bulk viscosity. Comparison of equations (18)-(21) with equation (17) shows that the expression in square brackets in equation (17) gives Cll, C~, K and (3/2)(C11- C12) if evaluated for the four loading cases. Additionally, C12 can be obtained from loading case (1), either by directly equilibriating the facet forces with a , or by superimposing the solution with ~11 :f=0, which is obtained from case (1) by an exchange of x I and x a. It remains to carry out the sum in equation (17) over the six square facets and the eight hexagonal facets of a tetrakaidekahedron to obtain the cubic viscosities.

3099

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING 5. RESULTS 5. I. The cubic viscosities The procedure described above leads to the cubic viscosities, which are given in dimensionless form according to

5.3. Comparison with an analytical estimate for K

kTR 3 Ciy = Cq f~ 6Dbp .

(22)

The same normalization is used for K and G. Table 4 shows the results. Apparently, the Cauchy relation, Cl2 = C44, is not fulfilled by the values shown in Table 4. This is because the forces on the facets are not independent but are coupled by the diffusion fluxes from one boundary to another. In the case of open porosity with isolated contacts the Cauchy relation is fulfilled [18]. In an isotropic material 2C44=Cl1-C~2. Inspection of Table 4 shows that the present model yields a strong cubic anisotropy. The factor 2 C ~ / ( C n - C12) varies from 5.5 for the fully dense material to 152 for rp/a =0.3x/2, while for an isotropic material the factor is 1. 5.2. Inclusion o f sliding forces So far grain boundary sliding was assumed to occur freely without any resistance. Now sliding forces as described by equation (5) are taken into account. To achieve this one notes that the contributions of normal and tangential forces on grain facets are additive in their effect on the cubic viscosities [18]. The contribution of tangential forces can be taken from the analysis of isolated grain contacts (equation (20) of [18]). Only the contact area needs to be adjusted to the situation of closed porosity. The total cubic viscosities are then

C12I| ~-- [-~ ~Dbp

c,4

\ c,,/

+ rIR(P°'~ '/3

[41-2 .

( - 2 In 09

33 --~+~o

o~2) --~-~

(24)

with co from equation (14). Table 5 shows a comparison between the bulk viscosities calculated numerically and those calculated from equation (24). The relative difference between the analytical and numerical results is small. It ranges from less than 2% for small porosities to about 10% for the largest pores considered. Hence, equation (24) can be used as a convenient approximation for the bulk viscosity. 5.4. lsotropic averages for G To obtain the isotropic shear viscosity the methods used in polycrystalline elasticity theory are applied, as in the case of open porosity [18]. The results are shown in Fig. 7 for the case that r / = 0 . As a consequence of the high anisotropy of the model the bounds lie considerably apart. Kr6ner's [20] self-consistent estimate, which lies between the Hashin-Shtrikman [21] bounds, is considered to be the best estimate. It is approximated by = 0.0300 - 0.0432rp/a

(25)

which is shown in Fig. 7 as a straight dashed line. The G / K ratio, calculated with the self-consistent estimate for G, has the values 0, 0.065, 0.116 and I

I

I

I

0.05

(23)

The first term arises from the normal forces with the Cu's from Table 4, while the second arises from the tangential forces. The voided area fraction of the square facets, ~o, was related to the density in equation (14). Table 4. Dimensionlesscubic viscositiesand bulk viscosity 0.05622 0.05448 0.04921 0.04038

kTR3 K = 618f~ Db~

<(.9

1+~33(1

0 ~ ov oo 0.1x~2 0.28166 0.27424 0.27671 0.2~2 0.13486 0.13199 0.13295 0.3,~2 0.05955 0.05902 0.05920

In [18] the bulk viscosity was estimated by assuming circular symmetric diffusive flow on all grain facets. The result was

0.06

-~o)

-a- \-~]

Table 5. Normalizedbulk viscositiesR = Kt'l fDbp/(kTR3). Comparison of an analyticalestimatewith the numericalresults rp/a = O.lx/2 0.2x/2 0.3x/2 R from equation (24) 0.282 0.139 0.065 /~ numerical 0.277 0.133 0.059

0.02050 0.00742 0.00287 0.00053

0 0.04 (/) > rr" 0.03' < I.U "10.02 n" 0.01 0 7, ( 0

C

1

1

_

~

~

~

0.1 0.2 0.3 0.4 NORM. PORE RADIUS rp/a

0.5

Fig. 7. Normalized cubic shear viscosities t ~ and ( ~ ' n - 6"12)/2 and estimates for the normalized isotropic shear modulus, t~. HS = Hashin-Shtrikman bounds [21].

3100

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING

0.197 for the values of rp/a = 0, 0.1x/2, 0.2x/2 and 0.3x/2, respectively. 5.5. Uniaxial creep without pores In order to compare the present results with those of Pan and Cocks [19] for creep of fully dense material, we consider uniaxial tension, i.e. the only nonzero stress component is 0-33. If one considers the case with tension along one of the cubic axes, one obtains the strain rate from equation (17) with 0- =0-33 and the term in square brackets = (3/2)(C11- Cl2), which is taken from Table 4. Then ~33= 272 f~ 6Dba33 k Td 3 •

(26)

Here the distance between opposite square facets, d, was used, which is related to R by d = (4/x/3)Rp~/3 for the fully dense material [from equation (12)]. Pan and Cocks [19] use the same quantities and obtain a numerical factor 153 instead of 272. (Their result in [22], a factor 554, was numerically incorrect.) With the self-consistent isotropic average of G, one obtains the uniaxial creep rate 0"33 ~'~ 6Dba33 ~33 = ~ = 88 kTd------T -

(27)

Coble's [23] classical analysis gave a numerical factor 148. A comparison of equations (26) and (27) shows that the cubic axes are exceptionally soft directions for tension, and the average creep rate is three times smaller. 6. INFLUENCE OF SURFACE DIFFUSION ON THE BULK VISCOSITY The pore shape was assumed in this paper to be the equilibrium shape consisting of spherical caps. This assumption is certainly justified if surface diffusion is very fast compared to grain boundary diffusion. However, a recent (theoretical) observation [24] indicated that an approximation based on equilibrium pore shapes yields results with a wide range of validity even for very slow surface diffusivities. In [24] sintering of a hexagonal array of wires was modelled numerically for arbitrary mean stresses, am, and for arbitrary ratios of 6Ds/rDb (where 6Ds is the surface diffusion coefficient). In analogy to cavity growth under tensile stresses [25] it was found that equilibrium pore shapes prevail, if the applied stress does not exceed a few times the sintering stress, nearly irrespective of the value of ~Ds/rDb. At higher compressive stresses and small 6DdrDb ratios, the material flowing out of the grain boundary into the pore forms extrusions. This is the analogue to the crack-like mode of cavity growth under high tensile stresses [25]. It appears that the range of validity of the equilibrium mode is larger under compressive than under tensile stress.

In [24] an additional important finding was made, which had not been discovered previously in connection with cavity growth. The numerical results for the pore shrinkage rates can be reproduced accurately by a quasi-equilibrium theory, which differs from the conventional equilibrium theory solely by the contribution of surface diffusion to the dissipation rate, which was previously neglected. This additional dissipative term may reduce the shrinkage rate by a large factor compared to the conventional equilibrium theory and it leads to accurate results (compared to the numerical solutions), as long as the pore shape globally resembles the equilibrium shape with possibly large deviations of the curvature near the pore tip. This condition of near-equilibrium shapes is fulfilled for nearly arbitrary 6Ds/6Db ratios, including very small ones, as long as the compressive stress does not exceed a few times the sintering stress. In situations of inhomogeneous sintering this prerequisite is always granted. There is no obvious reason that this quasiequilibrium theory, which was verified in [24] for a two-dimensional problem, should not be applicable analogously to the present three-dimensional problem. The shrinkage rate is derived from the thermodynamic principle that the negative rate of change of the Gibbs free energy must be equal to the dissipation rate due to the diffusive fluxes. The rate of change of the Gibbs free energy is, for hydrostatic loading -- (~tot

=

3 Vain Em -- 2ys f rVn dS alas

-- 6(2x/~+ 1)a2gmyb. (28) The first term results from the work rate of the macroscopic stress, the second accounts for the change of the surface area and of the grain boundary area due to the pore shrinkage, and the third describes the change of the energy of the grain boundaries surrounding the shrinking unit cell as pointed out in Section 3. The integral extends over the pore surface area pertaining to one grain, and vn is the velocity of the pore surface away from the center of curvature due to the plating or removal of material. The formulation of the capillary terms in equation (28) is an equivalent alternative to the formulation in Section 3. Within the quasi-equilibrium approximation, the integral on the pore surface is evaluated in the same way as in the equilibrium theory, namely by setting x =const, so that the integral becomes S xvn dS = xl?, and the sintering stress is obtained in exactly the same form as in the equilibrium theory, equation (9). As shown in [24] for the two-dimensional case this approximation leads to accurate results for the sintering rate in a wide range of conditions. The equality of the negative rate of the free energy and the dissipation rate gives 3 V(0-m -- as)~m = Rb + Rs

(29)

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING where Rb and Rs are the contributions of grain boundary diffusion and surface diffusion to the dissipation rate. The evaluation of the dissipation rates is described in the Appendix. The bulk viscosity is obtained as a sum of two terms, one arising from grain boundary diffusion K b, and the other from surface diffusion Ks

kTR3 ( ~Db ~ "~ Ktot=f~rObp ",/(b+ ~D~ K~)

where the hat indicates the normalized quantities, as before. The first contribution was given in Table 4, or, approximately by equation (24), while the latter is derived in the Appendix with the result

I(s= go + gl~o + g2o)2

configuration on the viscosities. F r o m their equation (44) one obtains the bulk viscosity, which in our notation is

~kTR3

K

108~ 6Dbp

{-2.45 ln(~)

-- 2.69 + 5.40(-~)2 - 3.53(-~)4]. (30)

(31)

3101

(35)

For spherical pores on the 24 grain corners, pore radius and relative density are related by r_p = a

(4 ; (1 - p)

.

(36)

Comparison of equations (24) and (35) shows that the bulk viscosity is about four times smaller for the

with

1

- 4 8 In cos ~ - 12 + 6 cos ~ + 14 cos 2 ~ - 9 cos 3 O + cos5

g0 (~b) =

g, (0) =

1

(2 + cos ~)2(1 - cos o)a

3 + cos ~k

18 (2 + cos ~O)(l + cos ~k)

1 2 + cos ~k g2(~O)- 144 (1 + cos ~O)2"

(33)

(34)

The g's are only moderately dependent on ~O. For ~k = 60 ° is go = 0.088, g) = 0.052, g2 = 0.0077. Also k s does not vary strongly with ff nor with ~o, and a typical value is k~ = 0.102 for q~ = 60 ° and co = 0.251. This is the same order of magnitude as/(b (which is 0.133 for ~o = 0.251 according to Table 4). Hence the contribution of surface diffsuion to the bulk viscosity can only be neglected, if 6Ds/fD b ~ 1, but it contributes substantially if 6Ds/fDb is of the order 1, and it dominates if 6Ds/fDb is small. As pointed out earlier, equation (30) can be expected to be a good approximation even for very small 6Ds/rDb(~. 1), unless the compressive stress becomes too large. More precise criteria for the range of validity are not yet available, but they can be developed in analogy to the analysis of cavity growth [25]. 7. DISCUSSION The preceding analysis of the densification and creep process was based on a specific grain and pore geometry with pores on the two-grain junctions between next-nearest grain neighbors. This geometry was motivated by a previous investigation on the evolution of equilibrium pore shapes [17], which indicated that this configuration is more likely to occur than the configuration with pores on the grain corners. The latter configuration was investigated by Pan and Cocks [19]. A comparison of their results with ours illustrates the influence of the pore

(32)

configuration with pores on the 24 grain corners than for that with pores on the six square facets; the comparison is made for the same relative density, and qJ = 90 ° is used, i.e. Fv---4 ~/3. Pan and Cocks [19] also consider the case of deviatoric creep in the [001] direction. Their result for the viscosities is, in our notation Cu - ~'~2= ~8 I0.209 - 4.41 ( ~ ) 2

Table 6 shows a comparison with our results for the same relative densities. The two models should agree for p = 1, when no pores are present in either model. The difference which actually occurs corresponds to the ratio 274/153 given previously and is probably due to the inaccuracy caused by the flow pattern assumed by Pan and Cocks for the deviatoric case. Once pores are present, the difference between the two models increases to about a factor 4 (for 0.3% porosity) and a factor 16 (for 8.5% porosity). It is not clear to what extent the difference is due to the different configurations or to inaccuracies of Pan and Cocks' estimate. No estimate for C44 nor for the isotropic average, G, is given by Pan and Cocks, so that no comparison is possible. Table 6. Valuesof 6"u - (?~2for two pore configurations;qJ = 90° is assumed p=l p=0.9969 p=0.9747 p=0.9152 Pan and Cocks 0.0365 0.0296 0.0177 0.00854 Present work 0.0205 0.0074 0.0029 0.00053

3102

RIEDEL et al.: DENSIFICATION IN THE FINAL STAGE OF SINTERING g. CONCLUSIONS

Densification and creep by grain b o u n d a r y diffusion are described by a linear viscous constitutive equation with compressibility and a sintering stress. The bulk and shear viscosities and the sintering stress are derived for a specific configuration of closed porosity. The diffusion problem is solved numerically using the finite element method. Since the assumed grain geometry, a tetrakaidekahedron, implies a b.c.c, symmetry, one primarily obtains cubic viscosity constants. F r o m the cubic viscosities the isotropic bulk viscosity, K, is easily obtained, since it is equal to the cubic bulk viscosity. A n analytical approximation for K [18] is confirmed, which shows that K diverges logarithmically, when full density is approached. To calculate the isotropic shear viscosity, G, the methods of polycrystaUine elasticity theory are applied. However, the result remains somewhat ambiguous, since, as a consequence of the pronounced anisotropy of the model, the H a s h i n - S h t r i k m a n bounds lie considerably apart. If the self-consistent method is assumed to give the best estimate, the G / K ratio drops from about 0.22 at pore closure to 0 at full density. The latter value is a necessary consequence of the fact that the material becomes incompressible. A comparison with an analysis of Pan and Cocks [19], who studied a different pore configuration, shows that the material becomes much more compliant (i.e. K and G drop), if the same pore volume is distributed on two times more, smaller and more closely spaced pores. Acknowledgement--The authors would like to thank the

Deutsche Forschungsgemeinschaft for financial support under contract Ri 329/18-1. REFERENCES 1. M. Abouaf, J. L. Chenot, G. Raisson and B. Baudin, Int. J. Num. Methods Engng. 25, 191 (1988). 2. J. L. Chenot, in Numerical Methods in Industrial Forming Processes, N U M I F O R M '89, (edited by E. G. Thompson, R. D. Wood, O. C. Zienkiewicz and H. Samuelson), pp. 11-16, A. A. Balkema, Rotterdam (1989). 3. A. Jagota, K. R. Mikeska and R. K. Bordia, J. Am. Ceram. Soc. 73, 2266 (1990). 4. K. Moil, in Numerical Methods in Industrial Forming Processes, N U M I F O R M '92, (edited by J. L. Chenot, R. D. Wood and O. C. Zienkiewicz), pp. 69-78. A. A. Balkema, Rotterdam (1992). 5. H. Riedel and D. Z. Sun, in Numerical Methods in Industrial Forming Processes, NUM1FORM "92 (edited by J. L. Chenot, R. D. Wood and O. C. Zienkiewicz), pp, 883486. A. A. Balkema, Rotterdam (1992). 6. A. C. F. Cocks and Z. Z. Du, Acta metall, mater. 41, 2113 (1993). 7. R. L. Coble, J. appl. Phys. 32, 787 (1961). 8. E. Arzt, Acta metall. 30, 1883 (1982). 9. A. S. Helle, K. E. Easterling and M. F. Ashby, Acta metall. 33, 2163 (1985). 10. A. G. Evans, J. Am. Ceram. Soc. 65, 497 (1982). 11. R. Raj and R. K. Bordia, Acta metall. 32, 1003 (1984).

12. C. H. Hsueh, A. G. Evans, R. M. Cannon and R. J. Brook, Acta metall. 34, 927 (1986). 13. R. K. Bordia and G. W. Soberer, Acta metall. 36, 2393 (1988). 14. G. W. Scherer, J. Non-Cryst. Solids 34, 239 (1979). 15. A. Jagota, P. R. Dawson and J. T. Jenkins, Mech. Mater. 7, 255 (1988). 16. R. M. McMeeking and L. T. Kuhn, Acta metall, mater. 40, 961 (1992). 17. J. Svoboda, H. Riedel and H. Zipse, Acta metall, mater. 42, 435 (1994). 18. H. Riedel, H. Zipse and J. Svoboda, Acta metall, mater. 42, 445 (1994). 19. J. Pan and A. C. F. Cocks, Acta metall, mater. 42, 1215 (1994). 20. E. Krrner, Z. Physik 151, 504 (1958). 21. Z. Hashin and S. Shtrikman, J. Mech. Phys. Solids 10, 343 (1962). 22. A. C. F. Cocks and J. Pan, in Creep and Fracture o f Engineering Materials and Structures (edited by W. Wilshire and R. W. Evans), pp. 41-51. The Institute of Materials, London (1993). 23. R. L. Coble, J. appl. Phys. 34, 1679 (1963). 24. J. Svoboda and H. Riedel, Quasi-equilibrium sintering for coupled grain-boundary and surface diffusion, IWM-Report M9/93, submitted to Acta metall, mater. 25. T.-J. Chuang, K. I. Kagawa, J. R. Rice and L. B. Sills, Acta metall. 27, 265 (1979). APPENDIX Evaluation o f the Dissipation Rate

It is the aim of this appendix to derive the contribution of surface diffusion to the bulk viscosity. The dissipation rate by grain boundary diffusion, Rb, need not be evaluated, since it leads to the bulk viscosity already derived in Sections 4 and 5 by other means. The dissipation rate by surface diffusion is defined as R, = - -

j~ dS

(AI)

where Js is the surface flux density and the integral extends over the six halves of the pores surrounding the unit cell. The surface flux that yields a sequence of equilibrium pore shapes with decreasing radius of curvature, r, is derived by considering the hatched volume shown in Fig. A1. In terms of the angle a, the hatched volume is v* = 5(2 - 2cose - sin2~ cos ~,)r 3.

(A2)

Its value changes by the surface flux entering the hatched volume and by the motion of the grains, the so-called jacking effect tl n

t)* = - 2 n r sin~js + ~- xr 2 sin2 ~.

(A3)

Fig. AI. Illustration of the calculation of the surface flux density.

RIEDEL et al.:

D E N S I F I C A T I O N IN THE FINAL STAGE OF SINTERING

Combining these equations gives the flux density j ~ = 2 I ( 2 cot ct - sin-~2 + sinct cos ~b)i + s i n f u l .

(A4)

The dissipation rate on the six half pore surfaces belonging to one grain is

6 k T f'~ 2 R~ = ~ [ j~2nr sin ~ d0c (A5) 0093o If j~ is inserted from equation (A4), one obtains R~ in the form R~--- ~ - ~ lloe + I ~ : 7 + I: (A6) ~.'OUs L z where the l ' s are integrals over ~t which can be evaluated in closed form I0 = - - 1 6 1 n c o s ~ - 4 +

+ 2cos ~ cos20-3cos 30+~cos50

(A7)

3103

16 2 I, = 2 - - - cos ff + 4 cos 2 ~k - ~ cos 4 ~b .3 3

(A8)

2 1 12 = ~ - cos tp + ~ cos 3 @.

(A9)

Only isostatic loading is considered here. Then t: and un are determined by the mean strain rate V~rn

t: = - 3F~r 2 Un =

(2 V) l/3~m.

(A10) (A 11)

Hence Rs oCg2m,and the contribution of surface diffusion to the bulk viscosity is K s = R~/(9V~2m) with Rs from equations (A6)-(A11). The result in the main text is obtained after r is expressed by rp through rp = r sin ¢, rp is replaced by a~/(to/n), a is expressed by the volume V of the grain, V is expressed by the grain radius R, combinations of the l ' s are formed to give the g's and equation (22) is used for the normalization of K.

Copyright © 2022 COEK.INFO. All rights reserved.